Hydrogen-evolution catalysts based on non-noble metal nickel-molybdenum nitride nanosheets.

Hydrogen production through splitting of water has attracted great scientific interest because of its relevance to renewable energy storage and its potential for providing energy without the emission of carbon dioxide. Electrocatalytic systems for H2 generation typically incorporate noble metals such as Pt in the catalysts because of their low overpotential and fast kinetics for driving the hydrogen evolution reaction (HER). However, the high costs and limited world-wide supply of these noble metals make their application in viable commercial processes unattractive. Several non-noble metal materials, such as transition-metal chalcogenides, carbides, and complexes as well as metal alloys have been widely investigated recently, and characterized as catalysts and supports for application in the evolution of hydrogen. Nitrides of early transition-metals have been shown to have excellent catalytic activities in a variety of reactions. One of the primary interests in the applications of nitrides in these reactions was to use them in conjunction with low-cost alternative metals to replace group VIII noble metals. For example, the function of molybdenum nitride as a catalyst for hydrocarbon hydrogenolysis resembles that of platinum. The catalytic and electronic properties of transition-metal nitrides are governed by their bulk and surface structure and stoichiometry. While there is some information concerning the effect of the bulk composition on the catalytic properties of this material, there is currently little known about the effects of the surface nanostructure. Nickel and nickel–molybdenum are known electrocatalysts for hydrogen production in alkaline electrolytes, and in the bulk form they exhibited exchange current densities between 10 6 and 10 4 Acm , compared to 10 3 Acm 2 for Pt. Jaksic et al. postulated a hypo-hyper-d-electronic interactive effect between Ni and Mo that yields the synergism for the HER. Owing to their poor corrosion stability, few studies in acidic media have been reported.With the objective of exploiting the decrease in the overpotential by carrying out the HER in acidic media, we have developed a low-cost, stable, and active molybdenum-nitride-based electrocatalyst for the HER. Guided by the “volcano plot” in which the activity for the evolution of hydrogen as a function of the M H bond strength exhibits an ascending branch followed by a descending branch, peaking at Pt, we designed a material on the molecular scale combining nickel, which binds H weakly, with molybdenum, which binds H strongly. Here we report the first synthesis of NiMo nitride nanosheets on a carbon support (NiMoNx/C), and demonstrate the high HER electrocatalytic activity of the resulting NiMoNx/C catalyst with low overpotential and small Tafel slope. The NiMoNx/C catalyst was synthesized by reduction of a carbon-supported ammonium molybdate [(NH4)6Mo7O24·4H2O] and nickel nitrate (Ni(NO3)2·4H2O) mixture in a tubular oven in H2 at 400 8C, and subsequent reaction with NH3 at 700 8C. During this process, the (NH4)6Mo7O24 and Ni(NO3)2 precursors were reduced to NiMo metal particles by H2, and then they were mildly transformed to NiMoNx nanosheets by reaction with ammonia. The atomic ratio of Ni/Mo was 1/4.7 determined by energy dispersive X-ray spectroscopy (EDX) on the NiMoNx/ C sample. The transmission electron microscopy (TEM) images, as shown in Figure 1a, display NiMo particles that are mainly spherical. The high-resolution TEM image, as shown in the inset of Figure 1a, corroborated the presence of an amorphous 3 to 5 nm Ni/Mo oxide layer (see Figure S4 in the Supporting Information for resolved image), whereas NiMoNx is characterized by thin, flat, and flaky stacks composed of nanosheets with high radial-axial ratios (Figure 1b and Figure S5 in the Supporting Information for a magnified image). Figure 1c shows that some of the nanosheets lay flat on the graphite carbon (as indicated by the black arrows), and some have folded edges that show different layers of NiMoNx sheets (white arrows). The thickness of the sheets ranged from 4 to 15 nm. The average stacking number of sheets measured from Figure 1b is about [*] Dr. W.-F. Chen, Dr. K. Sasaki, Dr. J. T. Muckerman, Dr. R. R. Adzic Chemistry Department, Brookhaven National Laboratory Upton, NY 11973 (USA) E-mail: ksasaki@bnl.gov